DOI: http://dx.doi.org/10.1590/1980-5373-MR-2015-0714Materials Research.
Graphite and Nickel Containing Tin Bronze-Steel Bimetals as Lead Free Bearing Materials
Ying Wanga, Qi Yanga*, Jintian Chenb, Jianping Zhoub
aSchool of Materials Engineering, Shanghai University of Engineering Science, Shanghai 201620, ChinabShanghai Hewei Corporation Limited, Shanghai 201615, China
Received: November 24, 2015; Revised: March 14, 2016; Accepted: May 7, 2016
Ni was added into graphite-lead free tin bronze composite layers on surface of steel sheets by primary sintering mixed powders of graphite and CuSn10 with addition of a nickel nitrate and poly(vinyl alcohol) (PVA) solution in an ammonia decomposition atmosphere. The reduced Ni particles attached on the surface of graphite and CuSn10 particles help to link them together. The conjunction of graphite and CuSn10 matrix in the composites treated by cold rolling and second sintering is well, and no cracks can be observed at the interface between graphite and CuSn10 matrix. The addition of Ni will improve the interface; increase hardness, anti-friction and anti-wear performance of the composites greatly. The Ni containing graphite-CuSn10 composites demonstrate better tribological performance than CuSn10Pb10 alloy, which makes them promising lead free bearing materials for heavy load engines.
Keywords: Tin bronze, Lead free, Graphite, Nickel, Composite
1. IntroductionLead tin bronze-steel bimetals were usually employed
as bearing materials of heavy load engines. Because of their high strength and thermal conductivity, the lead tin bronze layers were used as friction pairs. Steel sheets will further increase the strength and carry capacity of bearing materials, and reduce the amount of expensive nonferrous metals. However, lead is a harmful heavy metal and limitation has been imposed on its usage. Presently, considerable researches have been focused on developing lead free bearing materials1.
CuSn10Pb10 is one of the most common used lead tin bronzes for heavy load engine bearing materials. Because lead is a soft phase, it serves as lubricant for the bearing materials. As an excellent solid lubricant, graphite was applied into copper matrix composites as replacement of lead to improve their anti-friction property2-7. But the interface binding between graphite and copper matrix is weak due to their incompatibility, which decreases the mechanical and tribological performance of the composites2-7. Modification techniques of graphite such as: Cu electroplating8,9, Cu electroless plating10,11, Ni electroplating12 and Ni electroless plating13-15 are effective routes to improve the interface. Neverthe-less, these modification techniques are complicated, expensive and cannot be employed in large scale production.
In this work, the possibility of replacement of CuSn10Pb10 alloy by graphite-CuSn10 composites was explored by comparing their tribological performance; a novel, simple, cost effective and large scale production technique was also presented to improve the interface between graphite and CuSn10 matrix.
2.1 Starting materialsCuSn10, CuSn10pb10 and graphite powders with a particle
size of ~50 m and SPCC steel sheets with a thickness of
1mm were provided by Shanghai Hewei Corporation Limited. The chemical compositions of the SPCC steel sheets are C: 0.07 wt%, Si: 0.10 wt%, Mn: 0.35 wt%, S: 0.011 wt% and P: 0.008 wt%. Ni(NO3)26H2O and PVA1788 purchased from Sinopharm Chemical Reagent Corporation Limited were used as received.
2.2 Sample preparationPowder metallurgy techniques illustrated in Figure 1
were performed to prepare Ni containing graphite-CuSn10 composite layers on the surface of steel sheets. The typical large scale production processes of lead tin bronze-steel bimetals were as follow: spreading powders on the surface of steel sheetsprimary sinteringcold rollingsecond sinteringflattening16.
* e-mail: email@example.com
Figure 1: Flow diagram of preparation processes for graphite-CuSn10 composites containing Ni
The solution of Ni(NO3)2 and PVA was prepared by dissolving 80 g Ni(NO3)26H2O and 5 g PVA in 100 g pure water. CuSn10 powders, graphite powders and the solution with weight rates of 100 : 1.33, 2.20, 2.81, 3.45 : 25 were
Wang et al.2 Materials Research
mixed. Uniform slurry obtained by stirring the mixture was dried at 100 oC for 6 h, and the produced porous bulks were crushed into powders for following processes.
The crushed powders were loosely spread on the surface of steel sheets to form a layer with a thickness of ~1 mm. After sintered in an ammonia decomposition atmosphere at 800 oC for 1 h, they transform to porous layers. Cold rolling with a 10% deformation rate and second sintering at 850 oC for 1 h in an ammonia decomposition atmosphere were performed to densify the porous layers.
The weight percentage content of graphite in the obtained composite layers is 1.29 wt%, 2.11 wt%, 2.68 wt% and 3.27 wt% (are roughly equivalent to volume percentage content of 5 vol%, 8vol%, 10 vol% and 12 vol%).
2.3 Characterization and testsThe microstructures and chemical compositions of
the samples were analyzed by S-3400 Scanning Electron Microscope (SEM) and its Energy Dispersive Spectrometer (EDS). The Brinell hardness of the coatings was tested, using a 62.5 kgf load, 30 s dwell time and a steel ball with a diameter of 2.5 mm. Tribological performance tests were carried out by UMT-3MT-220 friction and wear testing instrument using a pin-on-disk technique. The size of samples was 50 mm10mm3 mm. The composite layers were taken as the plates. The spherical pins with a diameter of 6 mm were made of quenched chromium steel with a Rockwell hardness of 60-63. In these tests, samples are ground up to grade 1200 abrasive paper, and their surface roughness was 0.10.02 Ra. Each friction pair was cleaned in acetone before and after wear tests. All friction and wear tests were performed under a fixed load of 200 N at a sliding speed of 1 m/min. Wear rate of the samples was defined as their weight loss suffered per unit sliding distance. An electronic balance having a resolution of 0.0001 g was used to measure the weight loss.
3. Results and discussionsThe aim of primary sintering in powder metallurgy
processes of bimetals is to make metal particles to be connected with each other and attached on surface of steel sheets to form porous layers for following processes. Actually, for the mixture of graphite and CuSn10 powders without addition of Ni(NO3)2 and PVA solution, they are still separated particles and cannot form porous layers after primary sintering because of the presence of graphite powders. By adding Ni(NO3)2 and PVA solution into the graphite and CuSn10 powders, the porous layers on the surface of steel sheets can be obtained. Comparing Figure 2a with Figure 2b, it can be observed that the dark graphite particle and gray CuSn10 particles have smooth surface for the powders mixture without addition of Ni(NO3)2 and PVA solution; after adding the solution into the powders mixture, some smaller particles with a size of 1-5m were loaded on the surface of the graphite particle and CuSn10 particles and help to link them together. EDS was conducted to analyze the chemical compositions of the smaller particles. From the EDS patterns of point A and point B in Figure 2b (Figure 2c and Figure 2d), the
chemical compositions of point A are C (57.51 wt%), Cu (17.01 wt%), Sn (13.58 wt%) and Ni (11.90 wt%), and the chemical compositions of point B are C (11.21 wt%), Cu (20.16 wt%), Sn (26.57 wt%) and Ni (42.06 wt%). The C element originates from graphite particle, Cu and Sn elements are assigned to CuSn10 particles, Ni element is attributed to the smaller particles on their surface. Because Ni(NO3)2 will transform to metal Ni at high temperature in reducing atmosphere, the smaller particles are metal Ni.
Figure 3 shows the formation of Ni particles on the surface of graphite and CuSn10 particles. After CuSn10 powders, graphite powders and solution of Ni(NO3)2 and PVA were stirred for a period of time, the solution of Ni(NO3)2 and PVA will form a film on the surface of CuSn10 and graphite particles. Being sintered in an ammonia decomposition atmosphere, the Ni(NO3)2 in the film will be decomposed to NiO, and then reduced to metal Ni. The obtained metal Ni tends to form sphere morphologies to minimize its surface energy. By this technique of Ni addition, the Ni particles on the surface of CuSn10 and graphite particles will increase their connection, achieve relatively uniform distribution of Ni in the mixed powders, and avoid the enrichment of graphite powders in the upper layer of the mixed powders which was caused by great difference density between CuSn10 and graphite.
After primary sintering, the loosely spreading powders will transform to porous layers on the surface of steel sheets. Subsequently, cold rolling and second sintering will further dense the porous layers. Figure 4a and Figure 4b show SEM images of densified graphite-CuSn10 composite layers with 10 vol% graphite and Ni addition. The gray part is CuSn10 matrix and the black part is graphite. The interface of graphite and CuSn10 matrix is well combined, no cracks can be observed there. Figure 4c and Figure 4d exhibit SEM images of graphite-CuSn10 layers with 10 vol% graphite and no Ni addition. Apparent cracks appear at the interface between graphite and CuSn10 matrix. Figure 4e shows the EDS pattern of point C (the interface between graphite and CuSn10 matrix) in Figure 4b. The chemical compositions of point C are C (54.95 wt%), Cu (35.98 wt%), Sn (5.43 wt%) and Ni (3.64 wt%), indicating the interface between graphite and CuSn10 matrix contents metal Ni which are attributed to the smaller metal Ni particles on